This content has been downloaded from IOPscience. Please scroll down to see the full text.

Download details:

IP Address: 89.202.245.164

This content was downloaded on 06/11/2013 at 11:21

Please note that terms and conditions apply.

### Competition between in-plane buckling and bending collapses in nanohoneycombs

View the table of contents for this issue, or go to the journal homepage for more 2012 EPL 98 16005

(http://iopscience.iop.org/0295-5075/98/1/16005)

Qiang Chen1_{and Nicola M. Pugno}1,2,3(a)

1_{Laboratory of Bio-Inspired Nanomechanics “Giuseppe Maria Pugno”, Department of Structural, Geotechnical}
and Building Engineering, Politecnico di Torino - I-10129, Torino, Italy, EU

2_{National Institute of Nuclear Physics, National Laboratories of Frascati - Via E. Fermi 40,}
I-00044, Frascati, Italy, EU

3_{National Institute of Metrological Research - Strada delle Cacce 91, I-10135, Torino, Italy, EU}
received 18 November 2011; accepted in ﬁnal form 24 February 2012

published online 30 March 2012

PACS 62.20.M – Structural failure of materials

PACS 61.43.Gt – Powders, porous materials PACS 61.46.-w – Structure of nanoscale materials

Abstract – The classical hexagonal honeycomb theory for the uniaxial loading case, developed by Gibson and Ashby, considers buckling of the cell walls parallel to one symmetry axis. In general, buckling may also occur in the cell walls inclined with respect to the two symmetry axes. Therefore, in this letter, under the uniaxial loading conditions, we derive the critical stresses of buckling and bending collapses of nanohoneycombs, for which the surface eﬀect is included. Furthermore, the competition between the two failure modes is studied. The present theory could be used to design new nanoporous materials, e.g., scaﬀolds for the regenerative medicine or energy-absorption materials.

Copyright c EPLA, 2012

Introduction. – Porous materials, which can be often found in Nature [1], have high mechanical eﬃciency and are widely used as modern materials; for instance, they are used as core materials in sandwich structures [2], common in aerospace engineering, or as energy-absorption materials to reduce the loading impact and improve the resistance to crushing [3]. The mechanical properties of a honeycomb, and in particular its failure mechanisms, are therefore of great interest to material scientists. A number of pioneering studies [4–11] analyzed its in-plane and out-of-plane mechanical behaviors (e.g., elastic buckling); for the in-plane deformation mechanism, the stress-strain curve [3,7,10] is described by the linear elastic, plastic plateau and densiﬁcation regions. Lee et al. [12] studied the mechanical behavior and deformation mechanism of a honeycomb composite at the temperature ranging from 25◦C to 300◦C. The classical approach was developed by Gibson and Ashby [10]. They systematically investigated elastic buckling, plastic and brittle collapses of the 2D hexagonal honeycombs for uniaxial and biaxial loading cases. In the uniaxial loading case, the classical prediction only considers the buckling of the cell walls parallel to one

(a)_{E-mail: [email protected]}

symmetry axis; in spite of this, buckling could occur ﬁrst in the inclined cell walls.

When the cell size comes down into the nanoscale, the surface eﬀect, due to the high surface-to-volume ratio [13,14], starts to play an important role in deter-mining the mechanical properties of the structure. Exten-sive works [15–18] studied the inﬂuence of surface eﬀect on linear elastic and plastic properties of nanomaterials.

Considering the above statements, here we develop a theory to determine the buckling competition between the inclined and parallel cell walls with respect to the symme-try axes (in the following text, we simply call them inclined and parallel cell wall, respectively) of nanohoneycombs, under the uniaxial loading condition. Moreover, we sepa-rately establish the criteria for the competition of failure modes between buckling and bending collapses in the two principal directions [19]. The present theory could be used to design new stronger and stiﬀer honeycomb nanomate-rials and in general to tune their mechanical response.

The surface eﬀect on Young’s modulus and the buckling of inclined columns. –

The surface eﬀect on Young’s modulus. As the struc-tural size reduces to nanoscale, the surface-to-volume

Qiang Chen and Nicola M. Pugno

Fig. 1: Schematic of an inclined column.

ratio increases and the surface eﬀect, induced by the surface atoms of the structure, dominates the mechanical behavior. A classical expression of surface stresses, basing on the energy method, has been derived for the linear-elastic body [14]:

τ_{ij}= τ_{ij}0 + S_{ij}: ε_{ij}, (1)
where, τ_{ij} is the 2-rank surface stress tensor, τ_{ij}0 is the
surface residual stress tensor, S_{ij} is the surface stiﬀness
matrix, ε_{ij} is the surface strain tensor and the symbol
“:” represents the inner product of tensors. For the
one-dimensional case, it can be expressed in a linear form [15]:

τs_{= τ}0_{+ E}s_{ε,} _{(2)}

where, τs is the surface stress, τ0 is the surface residual stress, Es is the surface Young’s modulus and ε is the surface strain.

To predict the eﬀective Young’s modulus Eeff, we apply Miller and Shenoy’s [20] approach:

Eeff
E = 1 +
Es
Et
6 + 2_{b}t
, (3)

where, E is the Young’s modulus without considering the surface eﬀect, Esis the surface Young’s modulus, whereas, t and b are the cross-sectional thickness and width of the cell wall, respectively.

Equation (3) obeys the simple linear scaling law [21]
Eeff_{E = 1 + αl}_{in}_{/L, l}_{in}_{representing a material intrinsic}
length, under which surface eﬀect plays an important role;
α is a dimensionless constant, which depends on the
geom-etry of the structural elements and their deformations and
L ≡ t. Note that the term in the bracket will be close to 6
if t b (plate) or 8 if t = b (square beam).

The buckling of inclined columns. Basing on the large deﬂection theory, Chang [22] derived the buckling formulas of inclined columns (ﬁg. 1) with diﬀerent boundary tions. A numerical factor β reﬂects the boundary condi-tions and it is deﬁned as

β2_{=}_{−ϕR}2 _{(4)}

with

ϕ = −(f_{sin θ}_{+ g}_{cos θ}_{),}

where R = l/r is the slenderness ratio; f= F/(AE) and
g_{= f}_{cot θ} _{are constraint forces acting in the vertical}

Fig. 2: (a) Geometrical parameters of a unit cell; (b) loading in the x-direction; (c) loading in the y-direction; (d) stress distribution on the cross-section of cell walls. The moments in each scheme are identical due to the lattice periodicity.

and horizontal directions at the deformable end, respec-tively; θ is the inclined angle made by the column and the horizontal line after the column’s deformation; l is the length of the column; r is the radius of gyration; F is the external force; A is the cross-sectional area; E is Young’s modulus.

Considering the inclined columns as ﬁxed at both ends, the eigenvalue equation with respect to β is [22]:

β2

R2cot2 θ + 2

1− cos β

β sin β −1 = 0. (5) For the sake of simplicity, when 50 < R < 500, β is consid-ered as a constant and equal to 8.669, because it has a minor change when θ varies in the range 15◦–75◦. Note that β = 8.669 (i.e., θ = 15◦) is conservative, compared with 8.986 when θ = 75◦. Rearranging eq. (4) and substi-tuting r =I/A into it, we ﬁnd the buckling load of the inclined columns at the initial state (θ= θ) as

F =β2EI sin θ

l2 , (6)

where I is the cross-sectional moment of inertia. Failure analysis in thex-direction. –

Buckling. As discussed before, the inclined cell walls
are columns clamped at both ends. In the x -direction
(ﬁg. 2(b)), the area, on which the external stress acts,
is k_{1}b(l_{2}+ l_{1}sin θ), where k_{1} is the number of unit cells,
b is the width of the cell wall, θ is the angle between the
inclined cell wall and the horizontal line, and l_{2}, l_{1}are the

σb
cr,1=
β E_{1}
12
cos θ
α + sin θ
t_{1}
l_{1} with α = l2/l1. (7)
Competition between buckling and bending failure. The
yield stress of the constituent material is denoted by
σ_{ys}, and the elastic-plastic stress distribution is shown in
ﬁg. 2(d); then, the related failure moment due to bending
is
M_{max,p}= σ_{ys}bt2_{1}
c
t_{1}
1− c
t_{1}
+2
3
1
2−
c
t_{1}
2
. (8)

According to Ashby and Gibson [4], the maximum bending
moment M_{max,1}= F_{1}l_{1}sin θ/2 of the cell wall is at its
two ends. Then, the critical condition for the competition
between elastic buckling and plastic collapse can be
obtained by setting

M_{max,p}= M_{max,1}. (9)
Thus, we ﬁnd the critical stress for plastic collapse:

σ_{cr,1}p =
2
c
t_{1}
1− c
t_{1}
+2
3
1
2−
c
t_{1}
2
σ_{ys}
(α + sin θ) sin θ
_{t}
1
l_{1}
_{2}
.
(10)
Accordingly, by comparing σ_{cr,1}b = σ_{cr,1}p , we ﬁnd the
crite-rion for the competition between buckling and bending
collapses in the x -direction as

_{t}
1
l_{1}
crit
=
48
c
t1
1− c
t_{1}
+2_{3}
1
2−
c
t_{1}
2
β2_{sin 2θ}
σ_{ys}
E_{1}eff. (11)
Failure analysis in the direction. – In the
y-direction (ﬁg. 2(c)), since the buckling collapse may take
place in both the inclined and parallel cell walls, the
analysis is diﬀerent from that for the x -direction. Here,
we ﬁrst consider the buckling competition between the
two types of cell walls.

Buckling competition between the inclined and parallel
cell walls. In this case, the inclined cell walls are treated
as those in the x -direction. The area, on which the external
stress acts, is 2k_{2}bl_{1}cos θ, where k_{2}is the number of unit
cells in the y-direction. Correspondingly, the number of
cell walls is 2k_{2}, thus, the equivalent force acting on each
inclined cell wall is F_{2}= σbl_{1}cos θ and the buckling stress
is obtained as
σ_{cr,2}(1) =β2E
eff
1
12 tan θ
_{t}
1
l_{1}
3
. (12)

reﬂects the boundary conditions. The external buckling stress, in the y-direction, is the minimum between the buckling stresses of the inclined and parallel cell walls:

σb

cr,2= min(σ(1)cr,2, σ(2)cr,2). (14)
Competition between buckling and bending
fail-ure. Similarly, the maximum bending moment
M_{max,2}= F_{2}l_{1}cos θ/2 of the beam is at its two ends.
Thus, the critical condition for the competition between
elastic buckling and plastic collapse can be obtained
through

M_{max,p}= Mmax,2; (15)
and the critical stress for plastic collapse is obtained as

σ_{cr,2}p =
2
c
t_{1}
1− c
t_{1}
+2
3
1
2−
c
t_{1}
2
σ_{ys}
cos2 θ
_{t}
1
l_{1}
2
.
(16)
Then, the competition between buckling and bending
collapses is described by setting σb_{cr,2}= σp_{cr,2}, i.e.,

_{t}
1
l_{1}
crit
= cos θ
min(σ(1)_{cr,2}, σ(2)_{cr,2})
2
c
t_{1}
1− c
t_{1}
+2
3
1
2−
c
t_{1}
2
σ_{ys}
.
(17)
Analytic results. – Here, we employ aluminum
as a case study; Young’s modulus is E = 75 GPa,
the surface Young’s modulus is Es= 2.45 N/m [20],
σ_{ys}= 4.3 GPa [23], t_{1}= 5 nm and b t_{1}. Accordingly, we
obtain E_{1}eff= 75.5 GPa. For the x -direction, the results of
the parametric analysis are reported in ﬁg. 3. Figure 3(a)
shows that the critical buckling stress decreases as
α increases, when the inclined angle θ is ﬁxed. This
is because the force acting on the inclined cell walls
increases with increasing α, under the same external
stress, and thus a constant buckling force of the cell
walls results in a smaller external stress for increasing α.
It also shows that the buckling stress decreases as the
inclined angle θ increases, when α is ﬁxed. As for the
competition between buckling and bending collapses,
the analytical result is reported in ﬁg. 3(b); we can see
that the criteria are symmetric with respect to θ = 45o,
for which the lowest critical value of t_{1}/l_{1} emerges; also
the load for fully plastic failure (c = 0) is higher than that
for brittle failure (c = t_{1}/2). This is because fully plastic
failure requires larger moments. Figure 3(c) provides a
schematic of the failure mechanisms.

Qiang Chen and Nicola M. Pugno

Fig. 3: (Colour on-line) (a) Critical buckling stress vs. θ inﬂuenced by α, for when t1/l1= 0.1; (b) critical value of t1/l1 for buckling and bending competing failures in the x -direction; (c) schematics of the failure modes reported in (b). Note that the black parts in (c) denote points subjected to bending failure.

Fig. 4: (Colour on-line) (a) Buckling stresses σ_{cr,2}(1) and σ_{cr,2}(2)
vs.θ, as a function of α; (b) critical value of t1/l1 for buckling
and bending competing failures; (c) schematics of the failure
modes for the caseα = 1/9 reported in (b). Note that the black
parts in (c) denote points subjected to bending failure.

If we consider t1/l1= 0.05, t1= t2= 5 nm, we ﬁnd
E_{2}eff= E_{1}eff= 75.5 GPa. For the y-direction, the analytic
results of buckling stress and t_{1}/l_{1} are reported in ﬁg. 4.
Figure 4(a) shows that buckling of inclined cell walls
takes place (for t_{1} = t_{2}) as the length ratio α decreases
and the failure-transition points (from σ_{cr,2}(1) to σ_{cr,2}(2)) move
forwardly to large angles; in particular, when α = 1/4 or
1/5, the buckling only occurs in the parallel cell walls.
This is because σ_{cr,2}(1) increases when θ increases and
σ_{cr,2}(2) increases when α decreases. Figure 4(b) shows that
decreasing t1/l1 leads to buckling. Besides, we can also
see that if α = 1/5, the competition is only between the
buckling of the parallel cell walls, as shown in ﬁg. 4(a),
and bending collapses of the inclined cell walls. For
α = 1/9 the buckling of inclined cell walls gets involved,
namely, the curve denotes a critical condition between the
buckling of inclined cell walls and its bending collapses
when θ < θ_{c} and that between the buckling of parallel cell

walls and bending collapses of the inclined cell walls when
θ > θ_{c}. Figure 4(c) provides a schematic of the failure
mechanisms (α = 1/9).

Compared with the classical honeycomb theory, our
analytical approach gives us an interesting result about
the failure transition of a nanohoneycomb under the
uniaxial loading case, governed by the parameter t1/l1.
The derivation includes the surface eﬀect, but it can be
neglected when the cross-sectional size t_{1} is larger than
∼100 nm [24].

Conclusions. – In this letter, under the uniaxial loading conditions, we have derived the buckling stress of the inclined cell walls in nanohoneycombs, which is not treated in the classical approach by Gibson and Ashby. Then, basing on the existing buckling and plastic-failure theory, the competition between these two plastic-failure mechanisms is studied, including the surface eﬀect peculiar of the nanoscale.

The present theory could be used to design new nanoporous materials, e.g., scaﬀolds for the regenerative medicine or energy-absorption materials.

∗ ∗ ∗

The research related to these results has received funding from the European Rearch Council under the European Union’s Seventh Framework Programme (FP7/2007–2013)/ERC Grant agreement No. 279985 BIHSNAM.

REFERENCES

[1] Seki Y, Schneider M. S. and Meyers M. A., Acta Mater.,53 (2011) 5281.

[2] Foo C. C., Chai G. B. and Seah L. K., Compos. Struct., 80 (2007) 588.

[3] Xue Z. Y. and Hutchinson J. W., Int. J. Numer. Methods Eng.,65 (2006) 2221.

[8] Papka S. D. and Kyriakides S., Int. J. Solids Struct., 35 (1998) 239.

[9] Papka S.D. and Kyriakides S., Acta Mater.,46 (1998) 2765.

[10] Gibson L. J. and Ashby M. F., Cellular Solids: Structure and Properties, 2nd edition (Cambridge University Press, Cambridge) 1997.

[11] Bhat B. T. and Wang T. G., J. Mater. Sci.,25 (1990) 5157.

[12] Lee H. S., Hong S. H., Lee J. R. and Kim Y. K., J. Mater. Sci.,37 (2002) 1265.

[13] Pavese M., Musso S. and Pugno N., J. Nanosci. Nanotechnol.,10 (2010) 4240.

[14] Cammarata R. C., Prog. Surf. Sci.,46 (1994) 1.

[19] Peng B., Pugno N. and Espinosa H. D., Int. J. Solids Struct.,43 (2006) 3292.

[20] Miller R. E. and Shenoy V. B., Nanotechnology, 11 (2000) 139.

[21] Duan H. L., Wang J, Karihaloo B. L. and Huang Z.
P._{, Acta Mater.,}54 (2006) 2983.

[22] Chang C. H., Lect. Notes Appl. Comput. Mech., 22 (2005) 93.

[23] Pastor-Abia L., Caturla M. J., SanFabian E., Chiappe G.and Louis E., Phys. Status Solidi C,6 (2009) 2119.

[24] Sohn Y. S., Park J., Yoon G., Song J., Jee S. W.,
Lee J. H., Na S., Kwon T._{and Eom K., Nanoscale Res.}
Lett.,5 (2010) 211.